# M n = (DP)m = (25,000)( g/mol) = 2.60! 10 6 g/mol

Size: px
Start display at page:

Download "M n = (DP)m = (25,000)(104.14 g/mol) = 2.60! 10 6 g/mol"

## Transcription

1 14.4 (a) Compute the repeat unit molecular weight of polystyrene. (b) Compute the number-average molecular weight for a polystyrene for which the degree of polymerization is 25,000. (a) The repeat unit molecular weight of polystyrene is called for in this portion of the problem. For polystyrene, from Table 14.3, each repeat unit has eight carbons and eight hydrogens. Thus, m = 8(A C ) + 8(A H ) = (8)(12.01 g/mol) + (8)(1.008 g/mol) = g/mol (b) We are now asked to compute the number-average molecular weight. Since the degree of polymerization is 25,000, using Equation 14.6 M n = (DP)m = (25,000)( g/mol) = 2.60! 10 6 g/mol

2 14.5 Below, molecular weight data for a polypropylene material are tabulated. Compute (a) the numberaverage molecular weight, (b) the weight-average molecular weight, and (c) the degree of polymerization. Molecular Weight Range (g/mol) x i w i 8,000 16, ,000 24, ,000 32, ,000 40, ,000 48, ,000 56, (a) From the tabulated data, we are asked to compute M n, the number-average molecular weight. This is carried out below. Molecular wt Range Mean M i x i x i M i 8,000-16,000 12, ,000-24,000 20, ,000-32,000 28, ,000-40,000 36, ,080 40,000-48,000 44, ,000-56,000 52, M n =! x i M i = 33, 040 g/mol (b) From the tabulated data, we are asked to compute M w, the weight-average molecular weight. Molecular wt. Range Mean M i w i w i M i 8,000-16,000 12, ,000-24,000 20, ,000-32,000 28, ,000-40,000 36, ,800

3 40,000-48,000 44, ,880 48,000-56,000 52, M w =! w i M i = 36,240 g/mol (c) Now we are asked to compute the degree of polymerization, which is possible using Equation For polypropylene, the repeat unit molecular weight is just m = 3(A C ) + 6(A H ) = (3)(12.01 g/mol) + (6)(1.008 g/mol) = g/mol And DP = M n m 33,040 g/mol = = g/mol

4 14.8 High-density polyethylene may be chlorinated by inducing the random substitution of chlorine atoms for hydrogen. (a) Determine the concentration of Cl (in wt%) that must be added if this substitution occurs for 5% of all the original hydrogen atoms. (b) In what ways does this chlorinated polyethylene differ from poly(vinyl chloride)? (a) For chlorinated polyethylene, we are asked to determine the weight percent of chlorine added for 5% Cl substitution of all original hydrogen atoms. Consider 50 carbon atoms; there are 100 possible side-bonding sites. Ninety-five are occupied by hydrogen and five are occupied by Cl. Thus, the mass of these 50 carbon atoms, m C, is just m C = 50(A C ) = (50)(12.01 g/mol) = g Likewise, for hydrogen and chlorine, m H = 95(A H ) = (95)(1.008 g/mol) = g m Cl = 5(A Cl ) = (5)(35.45 g/mol) = g Thus, the concentration of chlorine, C Cl, is determined using a modified form of Equation 4.3 as C Cl = m Cl m C + m H + m Cl x 100 = g g g g! 100 = 20.3 wt% (b) Chlorinated polyethylene differs from poly(vinyl chloride), in that, for PVC, (1) 25% of the side-bonding sites are substituted with Cl, and (2) the substitution is probably much less random.

5 14.13 Make comparisons of thermoplastic and thermosetting polymers (a) on the basis of mechanical characteristics upon heating, and (b) according to possible molecular structures. (a) Thermoplastic polymers soften when heated and harden when cooled, whereas thermosetting polymers, harden upon heating, while further heating will not lead to softening. (b) Thermoplastic polymers have linear and branched structures, while for thermosetting polymers, the structures will normally be network or crosslinked.

6 14.14 (a) Is it possible to grind up and reuse phenol-formaldehyde? Why or why not? (b) Is it possible to grind up and reuse polypropylene? Why or why not? (a) It is not possible to grind up and reuse phenol-formaldehyde because it is a network thermoset polymer and, therefore, is not amenable to remolding. (b) Yes, it is possible to grind up and reuse polypropylene since it is a thermoplastic polymer, will soften when reheated, and, thus, may be remolded.

7 14.22 Explain briefly why the tendency of a polymer to crystallize decreases with increasing molecular weight. The tendency of a polymer to crystallize decreases with increasing molecular weight because as the chains become longer it is more difficult for all regions along adjacent chains to align so as to produce the ordered atomic array.

8 15.2 Compute the elastic moduli for the following polymers, whose stress-strain behaviors may be observed in the Tensile Tests module of Virtual Materials Science and Engineering (VMSE): (a) highdensity polyethylene, (b) nylon, and (c) phenol-formaldehyde (bakelite). How do these values compare with those presented in Table 15.1 for the same polymers? The elastic modulus is the slope in the linear elastic region (Equation 6.10) as E =! "! # = " 2 \$ " 1 # 2 \$ # 1 Since all the stress-strain curves pass through the origin, we make take σ 1 = 0 and ε 1 = 0. Determinations of σ 2 and ε 2 are possible by moving the cursor to some arbitrary point in the linear region of the curve and then reading corresponding values in the Stress and Strain windows that are located below the plot. (a) For high-density polyethylene, we selected σ 2 = 6.0 MPa with its corresponding ε 2 = Therefore, E =! 2 "! 1 # 2 " # 1 = 6.0 MPa " 0 MPa " 0 = 395 MPa = GPa The elastic modulus (average) for high-density polyethylene given in Table 15.1 is 1.08 GPa, which is significantly higher than this value. (b) For nylon, we selected σ 2 = 24.3 MPa with its corresponding ε 2 = Therefore, E =! 2 "! 1 # 2 " # 1 = 24.3 MPa " 0 MPa " 0 = 2860 MPa = 2.86 GPa The elastic modulus range for nylon 6,6 given in Table 15.1 is 1.58 GPa to 3.80 GPa; therefore, the value for the VMSE nylon lies within this range.

9 (c) For phenol-formaldehyde (bakelite), we selected σ 2 = 33.0 MPa with its corresponding ε 2 = Therefore, E =! 2 "! 1 # 2 " # 1 = 33.0 MPa " 0 MPa " 0 = 4850 MPa = 4.85 GPa The elastic modulus range for the phenol-formaldehyde given in Table 15.1 is 2.76 GPa to 4.83 GPa; therefore, this value for the VMSE phenol-formaldehyde lies just above the maximum value for this range.

10 15.3 For the nylon polymer, whose stress strain behavior may be observed in the Tensile Tests module of Virtual Materials Science and Engineering (VMSE), determine the following: (a) the yield strength, and (b) the approximate ductility, in percent elongation. How do these values compare with those for the nylon material presented in Table 15.1? (a) The yield strength corresponds to the first maximum (just beyond the initial linear-elastic region) of the stress-strain curve. This reading in the stress window located below the plot as the curser point is dragged along the stress-strain curve is 84 MPa. (b) The approximate percent elongation corresponds to the strain at fracture multiplied by 100 (i.e., 44.5%) minus the maximum elastic strain (i.e., value of strain at which the linearity of the curve ends multiplied by 100 in this case about 4%); this gives a value of about 40%EL. For nylon 6,6, the range of values of yield strength presented in Table 15.1 is 44.8 MPa to 82.8 MPa; therefore, the value for the VMSE nylon lies slightly above the upper value. The ductility range for nylon 6,6 is 15%EL to 300%EL; therefore, our value (40%EL) lies within this range.

11 15.8 On the basis of the curves in Figure 15.5, sketch schematic strain time plots for the following polystyrene materials at the specified temperatures: (a) Amorphous at 120 C (b) Crosslinked at 150 C (c) Crystalline at 230 C (d) Crosslinked at 50 C (a) Amorphous polystyrene at 120 C behaves a rubbery material (Figure 15.8, curve C); therefore, the strain-time behavior would be as Figure 15.5c. (b) Crosslinked polystyrene at 150 C behaves as a viscoelastic material (Figure 15.8, curve B); therefore, the strain-time behavior will be as Figure 15.5c. (c) Crystalline polystyrene at 230 C behaves as a viscous liquid (Figure 15.8, curve A); therefore, the strain-time behavior will be as Figure 15.5d. (d) Crosslinked polystyrene at 50 C behaves in a glassy manner (Figure 15.8, curve B); therefore, the strain-time behavior will be as Figure 15.5b.

12 15.11 For thermoplastic polymers, cite five factors that favor brittle fracture. For thermoplastic polymers, five factors that favor brittle fracture are as follows: (1) a reduction in temperature, (2) an increase in strain rate, (3) the presence of a sharp notch, (4) increased specimen thickness, and (5) modifications of the polymer structure

13 15.13 In your own words, describe the mechanisms by which semicrystalline polymers (a) elastically deform and (b) plastically deform, and (c) by which elastomers elastically deform. (a) and (b) The mechanisms by which semicrystalline polymers elastically and plastically deform are described in Section (c) The explanation of the mechanism by which elastomers elastically deform is provided in Section 15.9

14 15.14 Briefly explain how each of the following influences the tensile modulus of a semicrystalline polymer and why: (a) Molecular weight (b) Degree of crystallinity (c) Deformation by drawing (d) Annealing of an undeformed material (f) Annealing of a drawn material (a) The tensile modulus is not directly influenced by a polymer's molecular weight. (b) Tensile modulus increases with increasing degree of crystallinity for semicrystalline polymers. This is due to enhanced secondary interchain bonding which results from adjacent aligned chain segments as percent crystallinity increases. This enhanced interchain bonding inhibits relative interchain motion. (c) Deformation by drawing also increases the tensile modulus. The reason for this is that drawing produces a highly oriented molecular structure, and a relatively high degree of interchain secondary bonding. (d) When an undeformed semicrystalline polymer is annealed below its melting temperature, the tensile modulus increases. (e) A drawn semicrystalline polymer that is annealed experiences a decrease in tensile modulus as a result of a reduction in chain-induced crystallinity, and a reduction in interchain bonding forces.

15 15.15 Briefly explain how each of the following influences the tensile or yield strength of a semicrystalline polymer and why: (a) Molecular weight (b) Degree of crystallinity (c) Deformation by drawing (d) Annealing of an undeformed material (a) The tensile strength of a semicrystalline polymer increases with increasing molecular weight. This effect is explained by increased chain entanglements at higher molecular weights. (b) Increasing the degree of crystallinity of a semicrystalline polymer leads to an enhancement of the tensile strength. Again, this is due to enhanced interchain bonding and forces; in response to applied stresses, interchain motions are thus inhibited. (c) Deformation by drawing increases the tensile strength of a semicrystalline polymer. This effect is due to the highly oriented chain structure that is produced by drawing, which gives rise to higher interchain secondary bonding forces. (d) Annealing an undeformed semicrystalline polymer produces an increase in its tensile strength.

16 15.21 Would you expect the tensile strength of polychlorotrifluoroethylene to be greater than, the same as, or less than that of a polytetrafluoroethylene specimen having the same molecular weight and degree of crystallinity? Why? The strength of a polychlorotrifluoroethylene having the repeat unit structure will be greater than for a polytetrafluoroethylene having the same molecular weight and degree of crystallinity. The replacement of one fluorine atom within the PTFE repeat unit with a chlorine atom leads to a higher interchain attraction, and, thus, a stronger polymer. Furthermore, poly(vinyl chloride) is stronger than polyethylene (Table 15.1) for the same reason For each of the following pairs of polymers, plot and label schematic stress strain curves on the same graph [i.e., make separate plots for parts (a), (b), and (c)]. (a) Isotactic and linear polypropylene having a weight-average molecular weight of 120,000 g/mol; atactic and linear polypropylene having a weight-average molecular weight of 100,000 g/mol (b) Branched poly(vinyl chloride) having a degree of polymerization of 2000; heavily crosslinked poly(vinyl chloride) having a degree of polymerization of 2000 (c) Poly(styrene-butadiene) random copolymer having a number-average molecular weight of 100,000 g/mol and 10% of the available sites crosslinked and tested at 20 C; poly(styrene-butadiene) random copolymer having a number-average molecular weight of 120,000 g/mol and 15% of the available sites crosslinked and tested at -85 C. Hint: poly(styrene-butadiene) copolymers may exhibit elastomeric behavior. (a) Shown below are the stress-strain curves for the two polypropylene materials. These materials will display the stress-strain behavior of a normal plastic, curve B in Figure However, the isotactic/linear will have a higher degree of crystallinity (since isotactic are more likely to crystallize than atactic/linear), and therefore, will have a higher tensile modulus and strength. Furthermore, the isotactic/linear also has a higher molecular weight which also leads to an increase in strength.

17 (b) Shown below are the stress-strain curves for the two polyvinyl chloride materials. The branched PVC will probably display the stress-strain behavior of a plastic, curve B in Figure However, the heavily crosslinked PVC will undoubtedly have a higher tensile modulus, and, also a higher strength, and will most likely fail in a brittle manner--as curve A, Figure 15.1; these are the typical characteristics of a heavily crosslinked polymer. (c) Shown below are the stress-strain curves for the two poly(styrene-butadiene) random copolymers. The copolymer tested at 20 C will display elastomeric behavior (curve C of Figure 15.1) inasmuch as it is a random copolymer that is lightly crosslinked; furthermore, the temperature of testing is above its glass transition temperature. On the other hand, since -85 C is below the glass transition temperature of the poly(styrene-butadiene) copolymer, the stress-strain behavior under these conditions is as curve A of Figure 15.1.

18

19

### Polymer Melt Rheology. Introduction to Viscoelastic Behavior. Time-Temperature Equivalence

Topics to be Covered Polymer Melt Rheology Introduction to Viscoelastic Behavior Time-Temperature Equivalence Chapter 11 in CD (Polymer Science and Engineering) Polymer Melt Rheology δ τ xy Newton s Law

### Materials Issues in Fatigue and Fracture

Materials Issues in Fatigue and Fracture 5.1 Fundamental Concepts 5.2 Ensuring Infinite Life 5.3 Finite Life 5.4 Summary FCP 1 5.1 Fundamental Concepts Structural metals Process of fatigue A simple view

### Lösungen Übung Verformung

Lösungen Übung Verformung 1. (a) What is the meaning of T G? (b) To which materials does it apply? (c) What effect does it have on the toughness and on the stress- strain diagram? 2. Name the four main

### Page 1. 6. Which hydrocarbon is a member of the alkane series? (1) 1. Which is the structural formula of methane? (1) (2) (2) (3) (3) (4) (4)

1. Which is the structural formula of methane? 6. Which hydrocarbon is a member of the alkane series? 7. How many carbon atoms are contained in an ethyl group? 1 3 2 4 2. In the alkane series, each molecule

### Types of Strain. Engineering Strain: e = l l o. Shear Strain: γ = a b

Types of Strain l a g Engineering Strain: l o l o l b e = l l o l o (a) (b) (c) Shear Strain: FIGURE 2.1 Types of strain. (a) Tensile. (b) Compressive. (c) Shear. All deformation processes in manufacturing

### Tiangang TM BW-10LD (622)

Tiangang TM BW-10LD Oligomeric Hindered Amine Light Stabilizer (HALS) Poly-(N-β-hydroxyethyl-2,2,6,6-tetramethyl-4-hydroxy-piperidyl-succinate) CAS number 65447-77-0 BW-10LD BW-10LD is a highly effective

### Injection Molding Handbook Herausgegeben von Tim A. Osswald, Lih-Sheng Turng, Paul Gramann

Injection Molding Handbook Herausgegeben von Tim A. Osswald, Lih-Sheng Turng, Paul Gramann ISBN-10: 3-446-40781-2 ISBN-13: 978-3-446-40781-7 Leseprobe Weitere Informationen oder Bestellungen unter http://www.hanser.de/978-3-446-40781-7

### EUROLAB 25 years. The role of metrology and testing to characterize materials and products. EUROLAB 25th Anniversary Seminar

EUROLAB 25 years The role of metrology and testing to characterize materials and products April 9, 2015, Odense Danmark 1 Origin of Conformity Assessment The New Approach for the European Economic Community

### Tensile fracture analysis of blunt notched PMMA specimens by means of the Strain Energy Density

Engineering Solid Mechanics 3 (2015) 35-42 Contents lists available at GrowingScience Engineering Solid Mechanics homepage: www.growingscience.com/esm Tensile fracture analysis of blunt notched PMMA specimens

### Chapter Outline: Phase Transformations in Metals

Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations

### HW 9. Problem 14.5. a. To Find:

HW 9 Problem 14.5. To Find: ( The number-verge moleulr weight (b The weight-verge moleulr weight ( The degree of polymeriztion for the given polypropylene mteril Moleulr Weight Rnge (g/mol x i w i 8,000

### TENSILE BEHAVIOUR OF OPEN CELL CERAMIC FOAMS

Original papers TENSILE BEHAVIOUR OF OPEN CELL CERAMIC FOAMS LUKÁŠ ŘEHOŘEK*, **, IVO DLOUHÝ*,**, ZDENĚK CHLUP* *Institute of Physics of Materials ASCR, Žižkova 22, 616 62 Brno, Czech Republic **Institute

### ITU Department of Mechanical Engineering. MANUFACTURING PROPERTIES of ENGINEERING MATERIALS Lecture Notes. Prof.Dr.Ahmet Aran

ITU Department of Mechanical Engineering MANUFACTURING PROPERTIES of ENGINEERING MATERIALS Lecture Notes Prof.Dr.Ahmet Aran 2007 CONTENTS 1. Engineering Materials and Their Properties 1.1. Classification

### Introduction to Tensile Testing

CHAPTER 1 Introduction to Tensile Testing TENSILE TESTS are performed for several reasons. The results of tensile tests are used in selecting materials for engineering applications. Tensile properties

### Module 34. Heat Treatment of steel IV. Lecture 34. Heat Treatment of steel IV

Module 34 Heat reatment of steel IV Lecture 34 Heat reatment of steel IV 1 Keywords : Austenitization of hypo & hyper eutectoid steel, austenization temperature, effect of heat treatment on structure &

### Unit 11 Practice. Name: Class: Date: Multiple Choice Identify the choice that best completes the statement or answers the question.

Name: Class: Date: Unit 11 Practice Multiple Choice Identify the choice that best completes the statement or answers the question. 1) Crystalline solids. A) have their particles arranged randomly B) have

### High Performance Polyamides Fulfill Demanding Requirements for Automotive Thermal Management Components

High Performance Polyamides Fulfill Demanding Requirements for Automotive Thermal Management Components David Glasscock Walter Atolino Gary Kozielski Marv Martens DuPont Engineering Polymers Because they

### Landmark Lesson Plan: Man and Materials through History

Landmark Lesson Plan: Man and Materials through History Grades: 9-12 Subject areas: Chemistry, Materials Science, Polymers and History Based on The Development of Bakelite, a National Historic Chemical

### FDM Part Quality Manufactured with Ultem*9085

FDM Part Quality Manufactured with Ultem*9085 A. Bagsik 1,2, V. Schöppner 1, E. Klemp 2 1 Kunststofftechnik Paderborn (KTP),Universität Paderborn, D-33102 Paderborn, Germany 2 Direct Manufacturing Research

### SEISMIC UPGRADE OF OAK STREET BRIDGE WITH GFRP

13 th World Conference on Earthquake Engineering Vancouver, B.C., Canada August 1-6, 2004 Paper No. 3279 SEISMIC UPGRADE OF OAK STREET BRIDGE WITH GFRP Yuming DING 1, Bruce HAMERSLEY 2 SUMMARY Vancouver

### Chemistry 2014 Scoring Guidelines

AP Chemistry 2014 Scoring Guidelines 2014 The College Board. College Board, Advanced Placement Program, AP, AP Central, and the acorn logo are registered trademarks of the College Board. Visit the College

Delrin ONLY BY DUPONT Module III acetal resin Design information Registered trademarks of E.I. du Pont de Nemours and Company The miracles of science is a trademark of E.I. du Pont de Nemours and Company

### KALPANA INDUSTRIES LTD. TECHNICAL DATA SHEET

1 KALPANA INDUSTRIES LTD. TECHNICAL DATA SHEET KI XL - 03 / KI-SC 10 TWO COMPONENT AMBIENT CURABLE POLYETHYLENE COMPOUND FOR INSULATION OF LOW VOLTAGE POWER CABLE DESCRIPTION : KI polyethylene compound

### Technology, Tehran Polytechnic, Iran. Technology, Tehran Polytechnic,Iran. Guimarães, Portugal

Cementitious Composites Reinforced With Polypropylene, Nylon and Polyacrylonitile Fibres H.R. Pakravan 1, a, M. Jamshidi 2, b,m. Latifi 3, c, F.Pacheco-Torgal 4, d 1 Department of Textile Engineering,

### OUT SIDE BACK COVER OUT SIDE FRONT COVER

OUT SIDE BACK COVER OUT SIDE FRONT COVER CONTENT IRPC OVERVIEW PETROCHEMICAL BUSINESS POLYOLEFINS PRODUCTS 8 HDPE 9 HDPE PIPE COMPOUND 10 PP HOMOPOLYMER 11 PP BLOCK COPOLYMER 12 PP RANDOM COPOLYMER 13

### 5. MECHANICAL PROPERTIES AND PERFORMANCE OF MATERIALS

5. MECHANICAL PROPERTIES AND PERFORMANCE OF MATERIALS Samples of engineering materials are subjected to a wide variety of mechanical tests to measure their strength, elastic constants, and other material

### CARBON/DYNEEMA INTRALAMINAR HYBRIDS: NEW STRATEGY TO INCREASE IMPACT RESISTANCE OR DECREASE MASS OF CARBON FIBER COMPOSITES

26 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES CARBON/DYNEEMA INTRALAMINAR HYBRIDS: NEW STRATEGY TO INCREASE IMPACT RESISTANCE OR DECREASE MASS OF CARBON FIBER COMPOSITES J. G. H. Bouwmeester*,

### PRODUCT / APPLICATION INFORMATION

Abstract This paper will discuss performance life testing and stability testing used for self-regulating heating cables. It will show how the techniques were developed and evolved from the 970 s to the

### Ph.D. Thesis. Péter Juhász. Crystallisation kinetics and morphology of propylene/α-olefin random copolymers. Supervisor: Károly Belina

Péter Juhász Crystallisation kinetics and morphology of propylene/α-olefin random copolymers Supervisor: Károly Belina Budapest University of Technology and Economics Department of Plastic and Rubber Technology

### EFFECT OF SEVERE PLASTIC DEFORMATION ON STRUCTURE AND PROPERTIES OF AUSTENITIC AISI 316 GRADE STEEL

EFFECT OF SEVERE PLASTIC DEFORMATION ON STRUCTURE AND PROPERTIES OF AUSTENITIC AISI 316 GRADE STEEL Ladislav KANDER a, Miroslav GREGER b a MATERIÁLOVÝ A METALURGICKÝ VÝZKUM, s.r.o., Ostrava, Czech Republic,

### Dissertation. zur Erlangung des akademischen Grades. Doktor-Ingenieurin (Dr.-Ing.) vorgelegt der. (Ingenieurwissenschaftlicher Bereich)

Investigations on Environmental Stress Cracking Resistance of LDPE/EVA Blends Dissertation zur Erlangung des akademischen Grades Doktor-Ingenieurin (Dr.-Ing.) vorgelegt der Mathematisch-Naturwissenschaftlich-Technischen

### Usak University Journal of Material Sciences journal homepage: http://uujms.usak.edu.tr

Usak University Journal of Material Sciences journal homepage: http://uujms.usak.edu.tr Research article Mechanical properties of bi axial glass fiber and pistachio shell reinforced polyester composites

### Specific volume of polymers. Influence of the thermomechanical history

Specific volume of polymers Influence of the thermomechanical history CIP-DATA LIBRARY TECHNISCHE UNIVERSITEIT EINDHOVEN Beek, Maurice H.E. van der Specific volume of polymers : influence of the thermomechanical

### Modelling of Contact Problems of Rough Surfaces

Modelling of Contact Problems of Rough Surfaces N. Schwarzer, Saxonian Institute of Surface Mechanics, Am Lauchberg 2, 04838 Eilenburg, Germany, Tel. ++49 (0) 3423 656639 or 58, Fax. ++49 (0) 3423 656666,

### Experiment 13: Determination of Molecular Weight by Freezing Point Depression

1 Experiment 13: Determination of Molecular Weight by Freezing Point Depression Objective: In this experiment, you will determine the molecular weight of a compound by measuring the freezing point of a

### CURRICULUM VITA OF DR. RAMAZAN KAHRAMAN

CURRICULUM VITA OF DR. RAMAZAN KAHRAMAN Head of the College of Engineering Requirements Unit Professor, Chemical Engineering Department Qatar University, P.O. Box 2713, Doha, Qatar. Tel: +974 4403-4124

### X-ray diffraction in polymer science

X-ray diffraction in polymer science 1) Identification of semicrystalline polymers and Recognition of crystalline phases (polymorphism) of polymers 2)Polymers are never 100% crystalline. XRD is a primary

### EFFECTS OF SALT WATER AGING ON THE POST- IMPACT BEHAVIOR OF POLYMERIC COMPOSITES

EFFECTS OF SALT WATER AGING ON THE POST- IMPACT BEHAVIOR OF POLYMERIC COMPOSITES David R. Veazie 1, S.W. Park 2, and Min Zhou 2 1 Department of Engineering, Clark Atlanta University, Atlanta, GA 3314,

### Influence of Consolidation and Forming Parameters in the Molding of Continuous Fibre Reinforced Thermoplastic Composites

similar to that encountered in the thermoforming of thermoplastic polymer sheets. Influence of Consolidation and Forming Parameters in the Molding of Continuous Fibre Reinforced Thermoplastic Composites

### Topics to be Covered. Elements of Step-Growth Polymerization. Branching Network Formation

Topics to be Covered Elements of Step-Growth Polymerization Branching Network Formation Chapters 1 & 2 in CD (Polymer Science and Engineering) Dawn of Understanding "I am inclined to think that the development

### Energy saving and environment

Energy saving and environment Metal Work SpA has always placed great emphasis on environmental issues, and now following creation of the Environmental Management System and receipt of UNI EN ISO 14001

### Technical Data Sheet

Februar, 2014 Technical Data Sheet PLA Polylactide Cas No. 9051-89-2 PLA is a thermoplastic resin derived from annually renewable resources Product Characteristics Typical Properties Value Unit Physical

### Factsheet. UP Resins

Factsheet UP Resins & you COMPOSITE MATERIALS UP RESINS What is a UP Resin? Unsaturated Polyester Resins (UP Resins) are durable, resinous polymers dissolved in styrene. They are used in combination with

### Volume 54 2009 Issue 2 MLCF AN OPTIMISED PROGRAM OF LOW-CYCLE FATIGUE TEST TO DETERMINE MECHANICAL PROPERTIES OF CAST MATERIALS

A R C H I V E S O F M E T A L L U R G Y A N D M A T E R I A L S Volume 54 2009 Issue 2 M. MAJ,J.PIEKŁO MLCF AN OPTIMISED PROGRAM OF LOW-CYCLE FATIGUE TEST TO DETERMINE MECHANICAL PROPERTIES OF CAST MATERIALS

### Case Study 3. Cynar Plastics to Diesel

Case Study 3 Cynar Plastics to Diesel Report for ZWSA Ricardo-AEA/R/ED58135 Issue Number 1 Date 02/07/2013 Disclaimer: This case study has been prepared by Ricardo-AEA Ltd for the exclusive use of Zero

### C. PROCEDURE APPLICATION (FITNET)

C. PROCEDURE APPLICATION () 495 INTRODUCTION ASSESSMENT OF SCC ASSESSMENT OF CORROSION FATIGUE STRESS CORROSION AND CORROSION FATIGUE ANALYSIS ASSESSMENT OF LOCAL THINNED AREAS 496 INTRODUCTION INTRODUCTION

### 2009-12-23 ICS: 93.160. Strengthening retrofitting of reinforced concrete structures by gluing of fibre reinforced polymeric fabrics (FRP fabrics)

36888 ежглеяис тгс йубеямгсеыс (теувос еутеяо) 20091223 ICS: 93160 150114010801:2009 H HELLENIC CHNICAL SPECIFICATION (FRP ) Strengthening retrofitting of reinforced concrete structures by gluing of fibre

### Part B 2. Allow a total of 15 credits for this part. The student must answer all questions in this part.

Part B 2 Allow a total of 15 credits for this part. The student must answer all questions in this part. 51 [1] Allow 1 credit for 3 Mg(s) N 2 (g) Mg 3 N 2 (s). Allow credit even if the coefficient 1 is

### G1RT-CT-2001-05071 D. EXAMPLES F. GUTIÉRREZ-SOLANA S. CICERO J.A. ALVAREZ R. LACALLE W P 6: TRAINING & EDUCATION

D. EXAMPLES 316 WORKED EXAMPLE I Infinite Plate under fatigue Introduction and Objectives Data Analysis 317 INTRODUCTION AND OBJECTIVES One structural component of big dimensions is subjected to variable

### Finite Element Analysis of RC beams retrofitted with Fibre Reinforced Polymers. Giuseppe Simonelli

Finite Element Analysis of RC beams retrofitted with Fibre Reinforced Polymers Giuseppe Simonelli 27/11/2005 2 Acknowledgements I wish to thank Professor Luciano Rosati for his unconditional trust and

### Differential Scanning Calorimetry DSC

Analyzing & Testing Differential Scanning Calorimetry DSC Technique, Instrument, Applications DSC 3500 Sirius DSC 3500 Sirius Principle of Operation Differential Scanning Calorimetry Differential Scanning

### Where Is My Lone Pair?

Where Is My Lone Pair? Goal: In this tutorial we'll learn how to determine which orbital contains a lone pair. This is important for resonance, conjugation, and aromaticity. To master this subject you'll

### ME 612 Metal Forming and Theory of Plasticity. 1. Introduction

Metal Forming and Theory of Plasticity Yrd.Doç. e mail: azsenalp@gyte.edu.tr Makine Mühendisliği Bölümü Gebze Yüksek Teknoloji Enstitüsü In general, it is possible to evaluate metal forming operations

### Thermal (2) Coefficient of er -50 C to 150 C ppm/ C (Typical) Dissipation (1) Factor TAN d @ 10 GHz (Typical) (8) 0.0015 (8)

1 ACMPSGQ42014_v5.indd 1 Custom Materials RT/duroid, TMM, XT/duroid, ULTRALAM High Frequency Laminates Dielectric Constant, er @ 10 GHz Process (1) Design (11) Dissipation (1) Factor TAN d @ 10 GHz Thermal

### B. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS

B. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS 40 INTRODUCTION HOW ARE INTEGRITY, SECURITY OR CRITICAL CONDITIONS ANALYSED IN A CRACKED STRUCTURE? FRACTURE MECHANICS Critical conditions

### Symmetric Stretch: allows molecule to move through space

BACKGROUND INFORMATION Infrared Spectroscopy Before introducing the subject of IR spectroscopy, we must first review some aspects of the electromagnetic spectrum. The electromagnetic spectrum is composed

### PLEXIGLAS SUNACTIVE GS. For a Better Feeling

PLEXIGLAS SUNACTIVE GS For a Better Feeling PLEXIGLAS SUNACTIVE GS For a Better Feeling A perfect tan and a feeling of wellbeing are two important sales factors for tanning beds. To enable you to convincingly

INTDUCTIN T LEWIS ACID-BASE CEMISTY DEINITINS Lewis acids and bases are defined in terms of electron pair transfers. A Lewis base is an electron pair donor, and a Lewis acid is an electron pair acceptor.

### Consumer Products Made with Industrial Biotechnology

s Made with Industrial Biotechnology Consumer Bread Potassium bromate, a suspected cancer-causing agent at certain levels, added as a preservative and a dough strengthening agent microorganisms produces

### COMPOSITE MATERIALS. Asst. Prof. Dr. Ayşe KALEMTAŞ

COMPOSITE MATERIALS Office Hours: Tuesday, 16:30-17:30 akalemtas@mu.edu.tr, akalemtas@gmail.com Phone: +90 252 211 19 17 Metallurgical and Materials Engineering Department CONTENT Composite Materials Metal

### 1. Introduction 2. 2. Different types of asphalt pavement interlayers 3. 3. Fibre-rovings for asphalt pavement interlayers 5

1 Contents 1. Introduction 2 2. Different types of asphalt pavement interlayers 3 3. Fibre-rovings for asphalt pavement interlayers 5 4. Reinforced asphalt pavement as a composite building material 6 5.

### MBA Polymers. Richmond, California. Use of Recovered Plastics in the Manufacture of Automobiles, Appliances & Electronic Equipment

MBA Polymers Richmond, California Use of Recovered Plastics in the Manufacture of Automobiles, Appliances & Electronic Equipment (Recycling of Mixed Plastics) Commercial Demonstration Reported Fall 1999

### STRENGTH AND DUCTILITY OF WELDED JOINTS SUBJECTED TO OUT OF PLANE BENDING

STRENGTH AND DUCTILITY OF WELDED JOINTS SUBJECTED TO OUT OF PLANE BENDING by Ivan Gomez Amit Kanvinde University of California, Davis Yu Kay Kwan Gilbert Grondin University of Alberta Final Report Presented

### TECHNICAL BRIEF Critical Point Drying

TECHNICAL BRIEF Critical Point Drying Document Number Issue 2 Page 1 of 9 Critical Point Drying Technical Brief November 2009 Quorum Technologies Ltd main sales office: South Stour Avenue Ashford Kent

### White Dwarf Properties and the Degenerate Electron Gas

White Dwarf Properties and the Degenerate Electron Gas Nicholas Rowell April 10, 2008 Contents 1 Introduction 2 1.1 Discovery....................................... 2 1.2 Survey Techniques..................................

### Applied virtual (VT) technology on bus superstructure roll-over tests

Applied virtual (VT) technology on bus superstructure roll-over tests VINCZE-PAP Sándor 1, CSISZÁR András 2 1 JÁFI-AUTÓKUT Engineering Ltd., H-1115 Budapest, Csóka u. 7-13., email: vincze_pap@jafi-autokut.hu

### Chapter 8 Maxwell relations and measurable properties

Chapter 8 Maxwell relations and measurable properties 8.1 Maxwell relations Other thermodynamic potentials emerging from Legendre transforms allow us to switch independent variables and give rise to alternate

### Elasticity and mechanical advantage in cables and ropes

IOP PUBLISHING Eur. J. Phys. 8 (007) 715 77 EUROPEAN JOURNAL OF PHYSICS doi:10.1088/0143-0807/8/4/011 Elasticity and mechanical advantage in cables and ropes MJO Shea Department of Physics, Kansas State

### MATERIALS:MAIN RESEARCH ACTIVITIES ENRICO ALBIZZATI

MATERIALS:MAIN RESEARCH ACTIVITIES ENRICO ALBIZZATI Milan, October 25th, 2004 The home of Pirelli Labs Pirelli Labs - Materials Innovation The building A former heavy industry site; Builded in the early

### CONCRETE SEGMENTAL RETAINING WALL SYSTEM

CONCRETE SEGMENTAL RETAINING WALL SYSTEM PART 1: GENERAL SPECIFICATIONS 1.01 Work Included A. Work shall consist of furnishing and constructing a Rockwood Classic 8 with PCS unit segmental retaining wall

### MATERIAL SAFETY DATA SHEET

MATERIAL SAFETY DATA SHEET WORLD PRECISION INSTRUMENTS EMERGENCY NUMBER 941/371-1003 1/800/535-5053 175 Sarasota Center Blvd DATE PREPARED: Sarasota, FL 34240 12/01/95 Rev 02 SECTION I CHEMICAL IDENTIFICATION

### Methoden moderner Röntgenphysik II: Struktur und Dynamik kondensierter Materie

Methoden moderner Röntgenphysik II: Struktur und Dynamik kondensierter Materie Vorlesung zum aupt/masterstudiengang Physik SS 2011 G. Grübel, M. Martins, E. Weckert et al. SemRm3, Physik, Jungiusstrasse

### Evaluation of Fiber-Reinforced Asphalt Mixtures Using Advanced Material Characterization Tests

Evaluation of Fiber-Reinforced Asphalt Mixtures Using Advanced Material Characterization Tests By Kamil E. Kaloush, Ph.D., P.E., Associate Professor Arizona State University Department of Civil and Environmental

### TIIA SMOLANDER STUDY OF POLYPROPYLENE FOR USE IN MOBILE PHONES, AS A FUTURE ECO-FRIENDLY MATERIAL. Master of Science Thesis

TIIA SMOLANDER STUDY OF POLYPROPYLENE FOR USE IN MOBILE PHONES, AS A FUTURE ECO-FRIENDLY MATERIAL Master of Science Thesis Examiners: Professor Minna Kellomäki and M.Sc. (Engineering) Mika Pelto Examiners

### PVA Fiber Reinforced Shotcrete for Rehabilitation and Preventative Maintenance of Aging Culverts

PVA Fiber Reinforced Shotcrete for Rehabilitation and Preventative Maintenance of Aging Culverts A final report submitted to the Alabama Department of Transportation Project 930-657 December 2008 Investigators:

### 2.5 Physically-based Animation

2.5 Physically-based Animation 320491: Advanced Graphics - Chapter 2 74 Physically-based animation Morphing allowed us to animate between two known states. Typically, only one state of an object is known.

### ABSTRACT 1. INTRODUCTION 2. DESCRIPTION OF THE SEGMENTAL BEAM

Ninth LACCEI Latin American and Caribbean Conference (LACCEI 11), Engineering for a Smart Planet, Innovation, Information Technology and Computational Tools for Sustainable Development, August 3-, 11,

### 10. Standards for materials used in plumbing systems

10. Standards for materials used in plumbing systems 10.1 Standards Standards are sets of rules that outline specification of dimensions, design of operation, materials and performance, or describe quality

### ELASTOCEM. Technical features. Applications. Two-component flexible, waterproofing and protective cementitious grout.

Two-component flexible, waterproofing and protective cementitious grout. 1504-2 PI-MC-IR Technical features Two-component grout, based on cements, selected aggregates, special additives and synthetic polymers

### Heart Rate and Exercise

Name Date Heart Rate and Exercise Computer 26 Heart rates increase during exercise. The heart rates of physically fit people increase less during exercise than those of less fit people. The heart rates

### Topology Optimization of Modified Piston, Bridge Structures and Subway Tunnel Problem

Topology Optimization of Modified Piston, Bridge Structures and Subway Tunnel Problem Akash Dhiman 1, Anadi Misra 2 1PG Student, Mechanical Department, College of Technology, GBPUAT Pantnagar, Uttarakhand-

### Specialty Engineered Materials for Wire & Cable

Industr y Over view Specialty Engineered Materials for Wire & Cable Developing innovative polymer solutions that help wire & cable manufacturers exceed consumer expectations, stand apart from their competition

### Behaviour of buildings due to tunnel induced subsidence

Behaviour of buildings due to tunnel induced subsidence A thesis submitted to the University of London for the degree of Doctor of Philosophy and for the Diploma of the Imperial College of Science, Technology

### How do we determine which molecule is more basic?

How do we determine which molecule is more basic? One way to determine is by considering molecules structure, because structure can affect basicity of a molecule. Let s start with this concept. Higher

### WHITE PAPER Fire & safety performance standards

WHITE PAPER Fire & safety performance standards Terminologies describing Fire Performance Terminologies describing Fire Performance often present a challenge to understand as how they apply to a cable

### ! # # % % & () +, & +,,. / 0 % 1 + + 0 % 1 + + 2) () 3

! # # % % & () +, & +,,. / 0 % 1 + + 0 % 1 + + 2) () 3 4 SEISMIC EVALUATION OF REDUCED WEB SECTION(RWS) MOMENT CONNECTIONS Konstantinos Daniel Tsavdaridis Assistant Professor of Structural Engineering

### CONFORMATIONAL ANALYSIS PRACTICE EXERCISES. 1) Draw a Newman projection of the most stable conformation of 2-methylpropane.

CONFORMATIONAL ANALYSIS PRACTICE EXERCISES 1) Draw a Newman projection of the most stable conformation of 2-methylpropane. 2) The structures below are: C 3 C 3 C 3 C 3 A) not isomers. B) conformational

### DIELECTRIC SPECTROSCOPY AS A DIAGNOSTIC TEST METHOD FOR THE DETERMINATION OF MECHANICAL DAMAGE IN MARBLE SAMPLES

The 10 th International Conference of the Slovenian Society for Non-Destructive Testing»Application of Contemporary Non-Destructive Testing in Engineering«September 1-3, 2009, Ljubljana, Slovenia, 415-421

### Tests and Analyses on Shear Strength Increment of Soft Soil under Embankment Fill

Tests and Analyses on Shear Strength Increment of Soft Soil under Embankment Fill Guanbao Ye Professor Key Laboratory of Geotechnical and Underground Engineering,Tongji University, Ministry of Education,

### Scientific Opinion on the safety evaluation of the process, PP crates CHEP, used to recycle plastic for use as food contact materials 1

SCIENTIFIC OPINION Scientific Opinion on the safety evaluation of the process, PP crates CHEP, used to recycle plastic for use as food contact materials 1 EFSA Panel on food contact materials, enzymes,

### Methods for Polymer Diagnostics for the Automotive Industry*

COMPONENT-ORIENTED TESTING 17 Methods for Polymer Diagnostics for the Automotive Industry* Wolfgang Grellmann and Beate Langer, Merseburg, Germany The further development from polymer testing to polymer

### Introduction to Hardness Testing

1 Introduction to Hardness Testing Hardness has a variety of meanings. To the metals industry, it may be thought of as resistance to permanent deformation. To the metallurgist, it means resistance to penetration.

### 60.12. Depend-O-Lok FxE Expansion Coupling. System No. Submitted By Spec Sect Para Location Date Approved Date. DEPEND-O-LOK FxE EXPANSION COUPLING

60.1 D-O-L FxE expansion couplings are a bolted, split-sleeve design that provides for expansion and contraction at the coupled joint. These couplings are furnished with restraint rings that, when affixed

### Genetic Algorithm. Based on Darwinian Paradigm. Intrinsically a robust search and optimization mechanism. Conceptual Algorithm

24 Genetic Algorithm Based on Darwinian Paradigm Reproduction Competition Survive Selection Intrinsically a robust search and optimization mechanism Slide -47 - Conceptual Algorithm Slide -48 - 25 Genetic

### Chapter 7: Polarization

Chapter 7: Polarization Joaquín Bernal Méndez Group 4 1 Index Introduction Polarization Vector The Electric Displacement Vector Constitutive Laws: Linear Dielectrics Energy in Dielectric Systems Forces

### COMPLETE REVISION May 2006. Process Industry Practices Piping. PIP PNCM0002 Piping Material Specifications Line Class Index

Piping Piping Specifications Line Index PURPOSE AND USE OF PROCESS INDUSTRY PRACTICES In an effort to minimize the cost of process industry facilities, this Practice has been prepared from the technical

### BEHAVIOR OF WELDED T-STUBS SUBJECTED TO TENSILE LOADS

BEHAVIOR OF WELDED T-STUBS SUBJECTED TO TENSILE LOADS R.A. Herrera 1, G. Desjouis 2, G. Gomez 2, M. Sarrazin 3 1 Assistant Professor, Dept. of Civil Engineering, University of Chile, Santiago, Chile 2